advertisement

A METHOD OF ESTIMATING MAXIMUM COARSE AGGREGATE VOLUME FOR SELF-COMPACTING CONCRETE BY MONTE-CARLO SIMULATION (Translation from Proceedings of JSCE, No.690/V-53, November 2001) Junpei OGIHARA Masashi NAKAI Toyoharu NAWA This paper proposes an estimating method of the coarse aggregate volume used for self-compacting concrete. This method employs a probability model derived by the Monte-Carlo simulation, which regards the critical state of self-compactability as a bridge structure of the coarse aggregate covered with adherent mortar films. The probability model was compared to the published results of previous experiments for examination and validation of its applicability. The comparison clarified that the application of the model would enable to estimate the coarse aggregate volume for self-compacting concrete and facilitate its mix design. Keywords: self-compacting concrete, self-compactability, volume of coarse aggregate, wall effect, Monte-Carlo simulation Junpei Ogihara is a stuff member in the Civil Engineering Department, Hokkaido Electric Power Co. Inc., Japan. He obtained his M. Eng. from the Muroran Institute of Technology in 1995. His research interests related to mix design of powder type self-compacting concrete using fly ash when he was a researcher in the Research and Development Department. He is a member of JSCE. Masashi Nakai is an assistant manager in the Kyogoku Hydropower Plant Construction Office, Hokkaido Electric Power Co. Inc., Japan. His research interests included mix design of powder type self-compacting concrete using fly ash when he was a senior researcher in the Research and Development Department. He is a member of JSCE. Toyoharu Nawa is an associate professor in department of structural and geotechnical engineering, Hokkaido University, Sapporo, Japan. He received his Dr.Engineering in 1992 from Tokyo Institute of Technology, Tokyo. He newly developed belite rich cement for high-strength and self-compacting concrete. His current research interests are fluidity and strength development for high performance concrete incorporating large volume of fly ash. He is a member of JSCE. - 167 - 1. INTRODUCTION Self-compacting concrete is generally regarded as special concrete in Japan, and its use has not yet become general practice [1]. This is partly because of its high price for delivery from ready-mixed concrete plants when compared with normal concrete [1],[2]. Cost reduction is therefore a key prerequisite for achieving widespread acceptance. One possible solution is to pursue labor saving in mixture design, while the use of recycled materials and simplification of production and quality control are other avenues to be explored. The authors have been conducting various studies to streamline the proportioning of self-compacting concrete made using fly ash from imported coal. This paper proposes a method of estimating the coarse aggregate content, a factor directly related to concrete quality, for labor-saving in the design of the concrete mix. 2. FACTORS AFFECTING MAXIMUM COARSE AGGREGATE CONTENT In design a mix for self-compacting concrete, determination of the coarse aggregate content takes top priority. This is because, assuming that concrete is a two-phase material consisting of coarse aggregate and mortar, self-compactability cannot be achieved unless the coarse aggregate content is below a certain limit, even if the mortar is proportioned so as to attain suitable rheological properties (such as yield value and plastic viscosity) [3],[4]. When the volume fraction of coarse aggregate exceeds this limit, the particles of coarse aggregate are prone to come into contact with each other, leading to bridging (interlocking) between obstacle, such as reinforcing bars [5]. The Architectural Institute of Japan (AIJ) proposes setting the unit bulk volume of coarse aggregate, Vg/Glim (Vg = unit absolute volume of coarse aggregate; Glim = solid volume percentage of coarse aggregate), in the range 0.50 to 0.55 m 3 /m 3 [6]. The Japan Society of Civil Engineers (JSCE), on the other hand, specifies a range of coarse aggregate content while limiting the minimum value of solid volume percentage [7]. Thus, it is known that the coarse aggregate content required to achieve self-compactability is closely related to the solid volume percentage of coarse aggregate. For a particular coarse aggregate content, the distance between aggregate particles is greater for an aggregate with a higher solid volume percentage [8], leading to lower risk of their coming into contact with one another as they pass through confined spaces. Matsuo et al. [9], however, point out that the ability to pass through a particular opening, as measured in V-funnel test, can be evaluated by Vg/Glim alone under normal circumstances, but that under when space is especially confined, the effect of particle size distribution should also be considered. The authors have obtained similar results in experiments on self-compactability using U-type testers (R1, R2), as described in a previous report [10], confirming that finer grading leads to improved self-compactability for a certain Vg/Glim value. In addition to grading, the maximum aggregate size, Gmax [11],[12], and particle shape [13] are also reported to affect self-compactability and the ability of concrete to pass through confined spaces. While solid volume percentage is considered a comprehensive index that incorporates these factors, the self-compactability of concretes having the same solid volume percentage of coarse aggregate may vary depending on the relative magnitude of the effects of these factors. Along with these considerations of spacing and aggregate quality, the limits of coarse aggregate content that achieve self-compactability may also depend on the fluidity and viscosity of mortar. It is therefore difficult to calculate the required coarse aggregate content only from the solid volume percentage. Instead, it is considered necessary to elucidate the relationships among all the above-mentioned factors and self-compactability. - 168 - With this as a background, a numerical simulation method is proposed in this paper for estimating the coarse aggregate content required to achieve self-compactability while handling the factors affecting self-compactability quantitatively. Concept of space blocking model Here, the authors assume the following basic conditions for their proposed space- blocking model based on the mechanism proposed by Fujiwara et al: Coarse aggregate particle Reinforcing bar Direction of concrete flow Fig.1 Behavior of coarse aggregate particles passing between reinforcing bars 200 280 20 200 CL 35 35 35 35 Type: R1 D10 490 Various efforts have been made to elucidate the relationship between concrete proportioning and ability to pass through confined spaces through experiments, theoretical analysis, and numerical analysis [14]. Among these, Fujiwara et al. [13] proposed a blocking model for investigating the ability of concrete to pass through confined spaces and thus estimate the maximum coarse aggregate content. They assume a bridging phenomenon of coarse aggregate particles between bars as illustrated in Fig. 1. As coarse aggregate particles pass through the space between reinforcing bars, they rotate on contact with the bars and thereby come into contact with other particles between the bars. If this contact leads to a stable structure, known as a bridge, concrete clogs the space. Fresh concrete 680 2.1 + + + + + 45 35 35 45 Type: R2 + + + + + + + + + + + + + + + + + + + + 190 + + + + + + + + + + + + R= 140 + + + + + + + + + Bh 50 1) The limit state of self-compactability is Reinforcing bars D13 assumed to be a state in which the fill height Bar obstacle in a U-type tester (Fig. 2) is 30 cm [7], which conditions occurs when coarse aggregate particles [in mm] Bh: Fill height covered with a mortar film form a bridge between reinforcing bars. The fill height may Fig.2 U-type tester also reach 30 cm in a case where the coarse aggregate segregates from the mortar, but this study only deals with situation in which no segregation occurs. The target slump flow is assumed to be as follows, in accordance with the JSCE Recommendations for Construction of Self-compacting Concrete (referred to as the JSCE Recommendations): - Maximum: 700 mm (650+50 mm) - Minimum: 500 mm (550-50 mm) + + + + + + + + + + 2) Concrete adhering to reinforcing bars is assumed to bind to the bars and not to flow. 3) Bridging occurs in a cross section of a space framed by pairs of reinforcing bars covered with a bound film of concrete (effective opening, Le × height, h). The effective opening, Le, is calculated from the thickness of the concrete film adhering to and bound to the bars, c, and the mean net opening between bars, Lo (Le = Lo – 2c). 4) The coarse aggregate particles are assumed to be ellipsoids expressed by an aspect ratio. 5) Coarse aggregate particles are assumed to move in a rotating motion with the diameter of rotation being the length of the ellipsoid. - 169 - Direction of concrete flow c c Le Concrete film adhering to and bound to bar t50 Reinforcing bar a a + 2t50 φ L0 Coarse aggregate (ｃ) Coarse aggregate particle covered with mortar film (Assumption of bridging particle) (a) Plan of bar obstacle (Assumption of Le) Vg lim = h t50 b + 2t50 b Rotating coarse aggregate particle φ Adhering mortar film ε= a δm = ( 1− ε- δm ) a/b Total area of in Fig. (b) h Le Total area of in Fig. (b) h Le a / b ：Mean aspect ratio of coarse aggregate Le = L0 − 2 c (b) Cross section of space between bars (Assumption of bridging structure) Fig.3 Concept of space blockage In this space blocking model, the coarse aggregate content in the limit state of self-compactability (at which the fill height of a U-type tester is 30 cm) is defined as the maximum coarse aggregate content, Vglim. The lower limit of Vglim in the 95% confidence interval, obtained by Monte-Carlo simulation as discussed later in this paper and used for mix design, is defined as the allowable maximum coarse aggregate content, Vglim’. Figure 3 illustrates the space blocking model. It is a two-dimensional representation of the limit state of self-compactability, in which coarse aggregate particles come into contact with bars in the grid area of a U-type tester, rotate, and form a stable structure (bridge) blocking the cross section of the space (effective opening, Le × height, h). Though Fujiwara et al. assumed that bridging occurs across the mean net opening between bars, Lo, we assume that it takes place across an effective opening, a width obtained by subtracting the concrete film thickness, c, from the mean net opening, Lo. Since bridging is assumed to result from rotation of coarse aggregate particles (ellipsoids with long and short axes a and b, respectively), that are covered in a mortar film to a thickness of t, followed by their coming into contact with one another, bridging in the cross section is described by circles of diameter a + 2t in apparent contact with one another. The maximum coarse aggregate content, Vglim, is therefore expressed as the ratio of the total area of ellipsoids to the cross-sectional area of the space, as given in Eq. (1). (1 − ε − δ m ) Vg lim = (1) a /b where Vglim = maximum coarse aggregate content (m 3 /m 3 ) - 170 - ε = void percentage of circular particles with a diameter of a + 2t in the cross-sectional space (Le × h) δ m = apparent percentage of adhering mortar in the cross-sectional space (Le × h) a b = mean aspect ratio of coarse aggregate In this equation, “ε” is calculated as a void percentage incorporating the size of the cross-sectional space, the thickness of mortar adhering to the aggregate particles, the particle size distribution of the coarse aggregate to which a Monte-Carlo simulation is applied, and the bridge structure. In the space blocking model, the coarse aggregate content required to achieve self-compactability decreases as ε and δ m increase and as the particle shape becomes flatter. The void percentage of granules and powder packed into a container is affected by the size and shape of the container. Particles become more difficult to pack as they near the walls of the container. This phenomenon, referred to as the wall effect in the field of powder engineering [15], causes the void percentage of a powder consisting of single-diameter particles to increase in containers with a smaller diameters. Accordingly, the void percentage of concrete given as Eq. (1) increases and Vglim decreases as the cross-sectional area of the space the concrete passes through decreases, even for identical coarse aggregate and mortar properties ( a b and δ m remain the same). On the other hand, Fujiwara et al. give the maximum coarse aggregate content (“χvt” in their original paper) as Eq. (2) using a different tester. Vg lim = where (1 − εmin ) a/b − ∆ Vg (2) εmin = void percentage by Horsfield’s closest packing configuration (εmin = 0.19 in the original paper) ∆ Vg = increment in coarse aggregate content in the center of net opening between bars Equation (2) separately calculates ∆ Vg due to the wall effect and the void percentage, εmin, by fixing them under certain conditions. However, the wall effect should normally be incorporated in the void percentage, and it is more reasonable to consider the void percentage as a complex function of grading, packing structure, and container size, since it depends on all these factors. The method of estimating the maximum coarse aggregate content proposed by the authors is based on the concept of Fujiwara’s blocking mechanism model but with a modified treatment of void percentage and incorporating the mortar properties and coarse aggregate grading. It can also be adapted to any obstacle conditions. The accuracy obtained is very good, as characterized by its suitability for statistical evaluation of the calculation results and ability to reflect variations in mortar properties. 2.2 Modeling of coarse aggregate particles a) Quantification of grading Most probabilistic events in the natural and social world are known to fit a normal distribution. In contrast, the peak of a powder grading curve tends to be shifted towards the fine side, giving an asymmetric distribution with a longer slope on the coarse side. The logarithmic-normal distribution and the Weilbull distribution (Rosin-Rammler distribution) with two parameters are frequently used to express this type of distribution 1 6 ) in the field of powder engineering. Though coarse aggregate is categorized as granular, the shape of its - 171 - distribution is considered to be similar to that of powder. A density function with a Weibull distribution [17] given by Eq. (3) is therefore adopted in this study. f(d′)= where p d′ θ θ p −1 d′p exp − θ (3) f(d’) = number-based density function d’ = d-5 (when the minimum size of the coarse aggregate is 5 mm) d = diameter of coarse aggregate (mm) p, θ = parameters Equation (3) is determined by parameters p and θ related to the shape and spread, respectively, of the density function. Since it is necessary to randomly generate particle diameters to fit any given size distribution in Section (5) of this Chapter, Eq. (3) ought to be a function based on the number of coarse aggregate particles. But with the size distribution measured in accordance with JIS A 1102 being produced from data based on particle mass, it does not agree with the distribution obtained by number-based measurement [16]. In order to obtain a number-based distribution, it is necessary to convert the mass data given by JIS A 1102 into number data using Eq. (4). It should be noted that this is an equation simplified to the degree possible without adversely affecting subsequent calculations; consequently, it is not meant to convert the mass in each size category into a precise number. fi = where Wi (4) ds i 3 fi = number of particles in size category i i = size category number (i = 1 to 4) when i = 1, size range of 5-10 mm when i = 2, size range of 10-15 mm when i = 3, size range of 15-20 mm when i = 4, size range of 20-25 mm Wi = mass fraction retained on a sieve of size category i (%) ds i = representative diameter in size category i (mm) when i = 1, ds 1 = 7.5 mm when i = 2, ds 2 = 12.5 mm when i = 3, ds 3 = 17.5 mm when i = 4, ds 4 = 22.5 mm The mean, µ , and standard deviation, σ , of a number-based particle size distribution can be determined by Eqs. (5) and (6), respectively, using Eq. (4). µ= 4 ∑ (ds i − 5) f i i =1 σ = 4 ∑ (ds i 4 ∑f (5) i i =1 − 5 − µ )2 f i i =1 4 ∑f (6) i i =1 From these equations, parameter p in Eq. (3) can be determined by solving Eq. (7) [18]. - 172 - 1 Γ 1 + p 1 Γ 1 + p 2 Γ 1 + − p However, Γ (s ) = ∫ ∞ 0 2 − σ =0 μ (7) x s −1e − x dx Since p is determined using Eq. (7), parameter θ can be determined from Eq. (8) [18]. θ= 1 1 Γ 1 + p μ (8) The parameters of Eq. (3) can thus be estimated. A goodness-of-fit test [19] should normally be carried out to investigate the number-based distribution is properly expressed by Eq. (3). However, such testing is not possible in this case as the present number of size categories is insufficient to allow checking with a χ 2 distribution given the degrees of freedom of the system, df (df = the number of size categories minus 1 – minus the number of parameters to be estimated). In order to carry out such a check, it would be necessary to increase the number of sieved size categories, but this is considered unrealistic at present time. Ma x len imum gt h M L Coarse aggregate M inimum length MW´ One method of quantifying particle shapes is to use the triple diameter. This is a method in which a particle is assumed to have three axes at right angles to each another. The long diameter, a, short diameter, b, and thickness, e, are measured along these axes, thereby defining the particle shape in terms of two diameter ratios, a/b and b/e. Though this type of three-dimensional specification is ideal, particle shape is quantified as a two-dimensional problem in this study in consideration of measurement simplification. The long and short diameters are measured from the projected sections. Per p ma endic xim u u m lar t o len gt h M W b) Quantification of particle shapes [20] Perpendicular to minimum length ML´ Fig.4 Method of measuring aspect ratio Care needs to be exercised in measuring the long and short diameters, because the aspect ratio depends on the order of measurement. The long diameter is measured first in this study, as shown in Fig. 4, as this assumes rotational motion of the coarse aggregate particles. Consequently, the aspect ratio is calculated according to Eq. (9). a/b= where 2.3 ML MW (9) a/b = aspect ratio ML = maximum length of coarse aggregate particle (= long diameter, a) MW =extent at right angles to the maximum length (= short diameter, b) Calculation of mortar film thickness on coarse aggregate The properties of concrete and mortar in self-compacting concrete are known to be expressible using a Bingham model using the yield value and plastic viscosity [21]. Kimura - 173 - et al. [22] assumed that concrete (the Bingham model) is a two-phase material consisting of mortar and coarse aggregate, and then calculated the mass of mortar adhering to an aggregate particle. Assumed that the aggregate particle was a sphere of diameter d, this mass of mortar is given by Eq. (10). Wm = where 5π d 2 τ m 6 102 (10) W m = mass of mortar adhering to one spherical particle (g) d = particle diameter (cm) τ m = yield value of mortar (Pa) According to experiments by Ohta [23], the surface area of coarse aggregate particles (crushed stone) is equivalent to 1.85 times that of a sphere of the same volume. To adapt this finding to the ellipsoidal assumption of this study, Eq. (10) is converted into Eq. (11) to calculate the mass of mortar adhering to an ellipsoid. W m ′ = 1 .85 where ( ) 5π ab 2 6 2 τm 3 (11) 102 W m ’ = mass of mortar adhering to one ellipsoid particle(g) a = long diameter (cm) b = short diameter (cm) τ m = yield value of mortar (Pa) If mortar is assumed to cover the surface of the ellipsoid to a uniform thickness t, then the volume of mortar adhering to one ellipsoid is given by Eq. (12). Vm ′ = where π 6 [(a + 2t )(b + 2t ) 2 − ab 2 ] (12) V m ’ = volume of mortar covering one ellipsoid a = long diameter (cm) b = short diameter (cm) t = thickness of mortar film (cm) From Eqs. (11) and (12), the film thickness of adhering mortar is given by Eq. (13). ( 9 .25 (ab ) − ) 4 t 3 + 2 (a + 2b )t 2 + 2 ab + b 2 t 2 2ω m where 2.4 2 3 τm 102 =0 (13) t = film thickness of mortar (cm) a = long diameter (cm) b = short diameter (cm) ω m = density of mortar (g/cm 3 ) τ m = yield value of mortar (Pa) Calculation of film thickness of concrete bound to reinforcing bars This scope of this investigation does not extend to situations in which coarse aggregate segregates from the mortar, so concrete that is not flowing is assumed to be bound (bonded) to the reinforcing bars, as in Fig. 3. The thickness of the concrete film, c, bound to a reinforcing bar is calculated from the equilibrium of forces acting on the bar surface as - 174 - φ given below. Since the flow velocity of concrete is assumed to be 0 cm/s at the bar surface, Eq. (14) is derived from the equilibrium of vertical forces acting on an infinitesimal area of the reinforcing bar surface, φ h/2 d α , as shown in Fig. 5. ω c dv = where τ cφh 2 dα φ/2 dα τcφh 2 dα α h ω c dv (14) ω c = density of concrete (g/cm 3 ) Fig.5 Forces acting on infin itesimal area o f rebar surface dv = infinitesimal volume of concrete bound to an infinitesimal area τ c = yield value of concrete (g/cm 2 ) φ = bar diameter (cm) h = bar length (cm) By integrating Eq. (14) with respect to α, the mass of concrete bound to bar is obtained using Eq. (15). ω cV c = where ∫ 2πτ cφh 2 0 (15) d α= πφh τc ω c Vc = mass of concrete bound to reinforcing bar (g) If it is assumed that the thickness of concrete bound to a reinforcing bar is constant at c, the volume of concrete bound to a single bar is given by Eq. (16). 2 2 φ φ Vc = πh + c − 2 2 where (16) Vc = volume of concrete bound to a single bar (cm 3 ) c = thickness of concrete film (cm) By substituting Eq. (15) into Eq. (16), the concrete film thickness is given by Eq. (17). c= where 1 4φ τc − φ φ2 + 2 ωc 102 (17) τ c = yield value of concrete (Pa) According to Komura et al. [24], the yield value of concrete is given by Eq. (18) if the concrete density is taken to be ω c = 2.3 g/cm 3 . τc = where 9 .12 Sf 2 × 10 7 (18) Sf = slump flow of concrete (mm) According to the JSCE Recommendations [7], more than 70% of self-compacting concrete is specified with a slump flow between 600 and 700 mm regardless of type. In this study, as - 175 - well, a slump flow of 600 mm is adopted; this simulates the more severe conditions for passage through the bars (small Le). The concrete film thickness was calculated from Eq. (17), while calculating τ c from Eq. (18) and assuming ω c to be 2.3 g/cm 3 . 2.5 Modeling of bridging of coarse aggregate particles covered in mortar film As explained in Section 2.1 of this Chapter, the limit state of self-compactability is assumed to be a stable bridging structure consisting of circular particles with a diameter of d + 2t in contact with one another in the two-dimensional cross section of a space framed with bars. It is therefore necessary to model the bridging of circular particles. The bridging structure is assumed to be a packed structure of circular particles, and the method of developing such a structure is described in this Section. a) Bridging structure assumptions The packing structure is known to vary depending on particle size, and the model shown in Fig. 6 has been proposed to explain differences packing structures [25]. This figure indicates that a particle of diameter D larger than a critical particle diameter Dc yields a packing structure different from the case where D<Dc. For particles with D>Dc, as shown in Fig. 6 D > Dc D < Dc (a), the action of gravity on the particles exceeds the (a) (b) inter-particle forces, such as bonding force and cohesive force, causing the particles to drop down Fig.6 Particle packing models into the mechanically most stable position, where they become densely packed. On the other hand, small light particles with D<Dc, as shown in Fig. 6 (b), are held at the point of first contact by inter-particle forces, and the resulting packing structure has a high void percentage. The critical particle diameter, Dc, represents the diameter at which the force of gravity acting on a particle equals the inter-particle force, and is thought to range from 30 to 50 µm. Since the coarse aggregate particles dealt with in this study are no smaller than 5 mm, the packing structure shown in Fig. 6 (a) is adopted for simulation. b) Method of producing assumed packing structure To model the random phenomenon of spherical particle packing, a Monte-Carlo simulation was adopted. This is a technique generally used to reproduce such random behavior as the packing of spherical particles using random numbers [26]. Among studies based on the Monte-Carlo technique, Ito et al. [27] simulated the packing of spherical particles having a discontinuous size distribution. The authors adopt the packing behavior proposed in this investigation, which results in a packing structure similar to that shown in Fig. 6 (a), and formulate a 2-D circular particle packing program by extending it to include continuous size distributions. The procedure for achieving packing is as follows: Circular particles are generated in conformity with the specified size distribution using Weibull quasi-random numbers and then placed in random positions (using uniform quasi-random numbers) above the packing layer. The particles are then allowed to fall vertically based on the following three assumptions: 1) Circular particles fall individually. 2) Circular particles do not bounce when they collide. 3) Packed circular particles do not move when a collision occurs. The falling particles are assumed to fall, until they come into contact with the packed particles, and then roll down to the most mechanically stable position, where they stop. - 176 - A A B A B (a) Particle A falls B (ｂ) Particle A comes into contact with Particle B (ｃ) ) Particle A rolls onto Particle B and settles Fig.7 Packing behavior of part icles Set packing range Figures 7 and 8 show the assumed packing behavior of particles and a flow chart of packing structure generation, respectively. Set Weibull quasi-random nu mbers for diameters of circu lar particles to be packed Set thickness of adhering mortar film, t 50 The programming language used for formulating the packing structure is Visual Basic 6.0 (Microsoft) [28],[29]. The Weibull quasi-random numbers are given by Eq. (19) [17]. 1 d ′ = θ− ( log e U ) p where Generate circular part icle according to Weibull quasi-random numbers (including diameter conversion in consideration of t 50 ) Place part icle at top of packing range according to uniform quasi-rando m numbers (19) d’=particle diameter generated by Weibull quasi-random numbers (mm) U = uniform quasi-random numbers in range (0, 1) p, θ = parameters in Eq. (3) Place part icle on the bottom Allow particle to fall vertically Contact with bottom Judge contact of the particle Contact with a packed particle Yes 2.6 Method of calculating maximum coarse aggregate content Figure 9 shows the calculation flow used to obtain the maximum coarse aggregate content by the Monte-Carlo method. The thickness of the mortar film used in the packing simulation of circular particles is assumed to be, t 5 0 , corresponding to mean diameter d 5 0 to simplify the calculation. The number of calculation trials for the packing simulation is 100 to improve the accuracy of the 95% confidence interval for Vglim. START Settled? No Roll part icle on the packed particle until it comes into contact with another surface (of packed particle, bar, or the bottom) Settled? No Yes Yes Is settled particle in the packing range? No Change the drop position according to uniform quasi-rando m nu mbers No Nu mber of changes to drop position > 500 Yes END Fig.8 Procedure fo r fo rming packing structure - 177 - Measure coarse aggregate grading Set the yield value and density of mortar Measure aspect ratio of coarse aggregate particles Identify parameters p and of Eq. (3) i =1 Simu late packing of circular part icles Generate particle d ia meter, d k ’ according to Eq. (19) and pack circu lar particles with diameters converted to Dk in the cross section (Le × h). The number of circu lar particles after co mpletion of packing is n Dk = d k′ + 5 + 2 t50 n 1 εi = 1 − Le h δm i = ∑ D= πDk2 k =1 1 n n ∑D Calcu late the thickness of the mortar film fro m Fig. (13) t50 Long diameter, a = mean d iameter, d 50 =μ+5 (μ： Eq .(5)) k k =1 /4 ( ) Set the packing range (space cross section) (width = Le, height = h) Le = L0 − 2 c 2 nπ 2 D − D − 2 t50 4 Le h PFi = 1 − εi − δm i Calcu late the concrete film thickness, c by Eq. (17) i = i +1 No i > 100 Yes Calcu late maximu m coarse aggregate content, Vglim PF = 1 100 Vg lim = 100 ∑ PF σ pf = i i =1 PF a/b ± Calcu late mean aspect ratio a / b 1.96 a/b 1 100 ∑ (PF − PF ) 100 2 Obstacle conditions of U-type tester L0 ：Mean net opening between bars φ：Bar diameter ｈ： Bar length (he ight of opening cross section) i i =1 σ pf Fig.9 Calculation procedure for maximu m coarse aggregate content 3. VERIFICATION OF SPACE BLOCKING MODEL The validity of the space blocking model is verified using test data taken from the literature. The input values for analysis with the model are as given in Table 1. Excepting the equalized concrete properties for setting the concrete film thickness, c, the input values match the original test conditions. Vglim is determined by following the calculation flow shown in Fig. 9. 3.1 Influence of coarse aggregate particle size distribution Figures 10 and 11 show test results previously reported by the authors [10], presented here to demonstrate that different particle size distributions can lead to different Vglim values yet achieve self-compactability. The maximum fill height in the U-type tester is set by changing the volumetric water-powder ratio, Vw/Vp, while keeping other proportions unchanged (Table 2), for each unit absolute volume of coarse aggregate, Vg. It should be noted that Vglim is assumed to be the coarse aggregate content corresponding to a maximum fill height according to the U-type tester, Bhmax, of 30 cm. Figures 12 and 13 show the grading and solid volume percentage, respectively, of the coarse aggregate used for the tests. - 178 - Table 1 Input values for analysis and their determination Inputvalues valuesfor foranalysis analysis Input Methodof ofdetermination determination Method Symbol Input Inputvalues valuesfor foranalysis analysis Symbol Sec.(1): Determine from measured Constants for probability Constants for probability Sec.(1): Determine from measured distribution densityfunctions functionsfollowing following distribution density thenumber-based number-basedsize size θ, , pp the θ Sec.(2):Estimate Estimatefrom fromfineness finenessmodulus modulus of of Sec.(2): distributionofofcoarse coarse distribution coarseaggregate aggregate coarse aggregate aggregate Film thickness of adhering thickness of adhering Substitute the following values into Eq. (13) ｔ ｔ5050 Film Substitute the following values into Eq. (13) mortar mortar Sec.(1): Estimate from measured mortar flow Sec.(1): Estimate from measured mortar flow τ Yield value of mortar τ mm Yield value of mortar Sec.(2): Input measured yield value of mortar Sec.(2): Input measured yield value of mortar ω Density of mortar ω mm Density of mortar Sec.(1), (2): Determine from mix proportions Sec.(1), (2): Determine from mix proportions Mean diameter of coarse Mean diameter of coarse d aggregate (in numberd 5050 aggregate (in numberbased size distribution) based size distribution) Sec.(1), (2): μ+ 5(mm); μ is determined Sec.(1), (2): μ+ 5(mm); μ is determined from Eq. (5) from Eq. (5) Table 2 Proportioning conditions Sec.(1): Input measured aspect ratio Sec.(1): Input measured aspect ratio Sec.(2): Estimate from solid volume Sec.(2): Estimate from solid volume percentage percentage Le Effective width of opening Calculate by assuming Le =L - 2c Le Effective width of opening Calculate by assuming Le =L00- 2c Mean net opening between L Mean net opening between Sec.(1), (2): Input bar obstacle conditions L 0 0 reinforcing bars Sec.(1), (2): Input bar obstacle conditions reinforcing bars Thickness of concrete film Sec.(1), (2): Determine from φ by Eq. (17) c Thickness of concrete film Sec.(1), (2): Determine from φ by Eq. 3(17) c bound to reinforcing bars assuming Sf = 600mm, ωc = 2.3 g/cm bound to reinforcing bars assuming Sf = 600mm, ωc = 2.3 g/cm3 Sec.(1), (2): Input bar obstacle conditions φ bar diameter Sec.(1), (2): Input bar obstacle conditions φ bar diameter h Space height Sec.(1), (2): Input bar obstacle conditions h Space height Sec.(1), (2): Input bar obstacle conditions condition: R1 D 300 300 E 250 250 F 200 200 150 150 Fine grain Fine 100 100 Coarse 粗粒 Coarse 5050 C G Vglim of Vglim coarse Vglim Vglim of of of coarse grain fine fine grain grain grain 00 0.26 0.34 0.28 0.36 0.30 0.38 0.32 0.40 0.340.42 0.360.44 0.38 0.32 3 3 Unit absolute volume of coarse aggregate, VgVg (m (m /m3/m ) 3) Unit absolute volume of coarse aggregate, Fig. 10 Relationship between unit absolute volume of coarse aggregate and maximum fill height (R1) Maximum fill height with U-type tester,Bhmax (mm) 350 350 Maximum fill height with U-type tester, Bhmax (mm) Maximum fill fill height height with with U-type U-type tester, tester, Bhmax Bhmax (mm) Maximum Obstacle condition: B ObstacleR2 A Wsp/Wp (％wt) Va （％） 50 45 1.5 6±1 400 400 350 350 300 300 B A H L D I E M 250 250 Obstacle Obstacle condition: condition:R2 R1 J F N 200 200 C K Fine grain Fine 150 150 Coarse 粗粒 Coarse 100 100 50 50 Vglim of Vglim coarse of coarse grain grain G Vglim Vglim of of fine fine graingrain 00 0.32 0.28 0.34 0.36 0.26 0.30 0.38 0.32 0.40 0.340.42 0.360.440.38 3 3 Unit absolute volume of coarse aggregate, Vg (m /m )3 3 Unit absolute volume of coarse aggregate, Vg (m /m ) Fig.11 Unit absolute volume of coarse aggregate (R2) 60 60 100 90 80 Solidvolume volumepercentage percentageofofcoarse coarse Solid aggregate,Glim Glim(%) (%) aggregate, Percentage passing by weight (%) Vs/Vm (％vol) Vf/Vg: Replacement ratio by volume of fly ash to Vs/Vm: Ratio by volume of fine aggregate to mor Wsp/Wp: Ratio by weight of superplasticizer to p Va: Air content Mean aspect ratio of a/b Mean aspect ratio of a/b coarse aggregate coarse aggregate 400 400 Vf/Vp (％vol) Fine grain 70 60 50 40 Coarse grain 30 Range of standard grading by JIS A 5005 20 10 5 10 15 20 25 Coarse grain Coarse i 58 58 57 57 Range of of FM FM Range corresponding to standard standard corresponding to grading by JIS JIS A A 5005 5005 grading by 56 56 6.4 6.6 6.8 7.0 7.2 6.4 6.6 6.8 7.0 7.2 Fineness modulus of coarse aggregate, FM Fineness modulus of coarse aggregate, FM 30 Nominal size of sieve opening (mm) Fig. 12 Grading of coarse aggregate Fine grain Fine grain 55 55 6.2 6.2 0 0 59 59 Fig. 13 Solid volume percentage of coarse aggregate - 179 - 2.5 Number-based probability density f(x) Number-based probability density, ｆ(d') 0.25 Fine grain （θ=3.57, p=1.63) 0.20 0.15 Coarse grain （θ=5.36, p=1.57) 0.10 0.05 Measurements（5-10mm） Measurements（10-25mm） 2.0 Probability density function （5-10mm） Probability density function （10‐25mm） 1.5 5-10mm（θ=0.429, p=1.27) 1.0 10-25mm（θ=0.425, p=1.70) 0.5 0.0 0.00 0 5 10 15 Particle diameter, d ' (mm) 0 20 1 2 3 a/b -1 Fig. 15 Measured aspect ratios and probability Fig. 14 Probability density function of grading density functions Comparisons between measured values of Vglim and those estimated using the space blocking model are discussed in the following sections. a) (i) Parameter setting for space blocking model Particle size distribution The particle size distribution of the coarse aggregate used in the analysis, as shown in Fig. 12, is converted into a number-based density function described in Chapter 2, Section (2). The result is shown in Fig. 14. (ii) Mean aspect ratio The aspect ratio of the coarse aggregate was measured using a digital camera as an image input device and a personal computer with commercially available software as an image analysis system. The aggregate particles were divided into two groups by size: 5-10 mm and 10-25 mm. Each group was photographed, and the long and short diameters of the images were measured on the PC using Power Point 97 (Microsoft). The aspect ratio was then calculated using Eq. (9). The number of randomly selected particle samples was 100 for each group. In previous experiments [10], fine-grain and coarse-grain concretes were mixed by including coarse aggregate particles at mass ratios of 55:45 and 20:80, respectively, from the 5-10 mm and 10-25 mm groups. The mean aspect ratios are calculated similarly here. In other words, the measured aspect ratio for each size group is applied to the probability density function of Eq. (3) for the Weibull distribution to quantify it. Figure 15 shows the measured data and the probability density function to which the measured data are applied. It should be noted that goodness-of-fit testing is carried out for each size group, and that goodness of fit is confirmed at a significance level of 5%. The mean aspect ratio used for the analysis is determined by generating random numbers conforming to the probability density function for each size group and taking samples from the aspect ratio distribution for each size group according to the number fraction to obtain 500 samples in total. The mean value is taken as the aspect ratio. It should be noted that all generated random numbers are proven to satisfy the 5% level of significance (frequency checking and serial correlation checking) [31],[32]. - 180 - 400 Fine grain（R1） Mortar flow of mixes attaining Bhmax, Fm(mm) Slump flow of mixes attaining Bhmax , Sf (mm) 750 Coarse grain（R1) 700 Fine grain（R2） Coarse grain（R2） 650 600 550 500 0.25 0.3 0.35 0.4 0.45 3 3 Unit absolute volume of coarse aggregate, Vg (m /m ) Coarse grain（R１） Fine grain（R2） 350 Coarse grain（R2） 300 250 200 0.25 0.3 0.35 0.4 0.45 3 3 Unit absolute volume of coarse aggregate, Vg (m /m ) Fig. 16 Relationship between unit absolute volume of coarse aggregate and slump flow of concrete (iii) Fine grain（R1） Fig. 17 Relationship between unit absolute volume of coarse aggregate and mortar flow Mortar properties Table 3 Cases of mix proportion The density and yield value of the mortar have to be established in order to quantify mortar properties. Figures 16 and 17 show the influence of unit absolute volume of coarse aggregate, Vg, on concrete slump flow and mortar flow (mortar wet-screened with a 5-mm sieve) shown in Figs. 10 and 11, respectively. The data in the figures represent the maximum values of slump flow and mortar flow obtained without segregation occurring. These figures demonstrate that a finer aggregate leads to a higher concrete slump flow than a coarse aggregate with the same Vg, regardless of obstacle conditions. The effect of aggregate on mortar flow is similar. Accordingly, finer grading of the coarse aggregate particles can lead to increased fluidity and improved self-compactability while avoiding segregation, eventually allowing for a higher maximum coarse aggregate content. Waterpowder ratio Ww/Wp (%wt) Sandmortar ratio Vs/Vm (%vol) 32.4 0.35～0.55 Unit absolute Dosage of Supervolume of plasticizer coarse Wsp/Wp aggregate (%wt) Vg (m3/m3) 0.25 0.28 0.30 1.5～1.9 Air content Va (%) 6±1 Table 4 Materials Material Normal portland cement Specifications Density: 3.16g/cm3, Specific surface area by blaine: 3,360cm2/g PR/BA coal (ignition loss: 1.8%, methylene blue adsorption: 0.64mg/g, Fly ash made from density: 2.13g/cm3, specific surface by imported coal Blaine: 2,790cm2/g, bulk density: 1.221g/cm3, packing ratio: 57.3%) Land sand from Hamaatsuma (SSD density: 2.70g/cm3, absorption: 2.13%, FM: 2.48, solid volume percentage: 65.5%) Aggregate Crushed stone 2005 from Teine (SSD density: 2.68g/cm3, absorption: 1.44%, FM: 6.84, solid volume percentage: 59.3%) Complex of polycarboxylic ether type Superplasticizer and crosslinking polymer Air content Air-entraining admixture (high adjuster alkylcarboxylate type) Since differences in mortar properties are assumed to result from variations in the particle size distribution, it is necessary to establish mortar properties for each size distribution. Another series of experiments is conducted to determine the relationship between flow and yield value of wet-screened mortar, as yield values were not covered by the previous experiments [10]. Tables 3 and 4 give the mix proportions of the concrete and the materials used, respectively. - 181 - Table 5 Mortar properties Grading Fine grain R1 Coarse grain Fine grain R2 Coarse grain Mixture Vg (m3/m3) A B C D E F G H I J K L M N 0.28 0.32 0.36 0.28 0.30 0.32 0.36 0.33 0.36 0.39 0.42 0.33 0.36 0.39 Quantity of material per unit volume of concrete (kg/m3) W C F S 172 302 218 805 166 276 199 756 160 252 182 707 161 319 230 805 156 309 223 780 151 299 216 756 163 246 177 707 159 279 201 744 160 252 182 707 151 239 172 671 143 226 163 634 154 287 207 744 142 280 202 707 151 239 172 671 The mixing method is the same as in the previous experiments [10]. Figure 18 shows the mortar flow versus yield value relationship, and the results of regression of this relationship are expressed as Eq. (20). Yield values are obtained using a rotational viscometer (HAAKE RS150 with vane sensors) under stress control (minimum stress = 0.05 Pa). (20) log 10 τ m = − 0 .0142 Fm + 5 .32 where τ m = yield value of mortar (Pa) Fm = mortar flow (mm) Mortar properties Density Mortar Yield value (Pa) (g/cm3) flow (mm) 2.08 316 7 2.05 291 15 2.03 300 11 2.10 300 12 2.10 292 15 2.09 278 24 2.02 310 8 2.06 313 8 2.03 303 10 2.02 311 8 2.01 306 9 2.08 305 10 2.08 298 12 2.02 306 9 10000 r = -0.977 Yield value of mortar, τm (Pa) Obstacle condition 1000 100 10 1 Vg=0.25(Sp/P=1.5) Vg=0.25(Sp/P=1.7) Vg=0.25(Sp/P=1.9) Vg=0.28(Sp/P=1.5) Vg=0.28(Sp/P=1.7) Vg=0.28(Sp/P=1.9) Vg=0.30(Sp/P=1.5) Vg=0.30(Sp/P=1.7) Vg=0.30(Sp/P=1.9) Regression line Table 5 gives the estimated density and 0.1 yield value of the mortar in the concrete of 100 150 200 250 300 350 400 Mortar flow, F m (mm) Figs. 10 and 11, as determined from the above results. For the analysis, the mean Fig. 18 Relationship between mortar flow and yield value property values of two mortar mixtures, one below and one above Vglim were selected for each of the obstacle conditions and grain types. (indicated by the hatched cells in Table 5), (iv) Selection of concrete film thickness The film thickness of concrete bound to reinforcing bars was calculated using Eq. (17) as follows: Obstacle conditions R1 (Lo = 35 mm, φ (bar diameter) = 10 mm): c = 6.5 mm Obstacle conditions R2 (Lo = 40 mm, φ = 13 mm): c = 7.0 mm b) Comparison of space blocking model and measurements Figures 19 and 20 compare measurements of Vglim with values estimated by the space blocking model. The analytical parameters are given in Table 6. Fine-grain mixtures yield higher Vglim values than coarse-grain mixtures, and Vglim decreases as the mean net opening decreases for both obstacle conditions. Absolute values of measured and estimated Vglim are also similar. The analytical values tend to indicate that the influence of grading on Vglim falls as the mean net opening increases, which is similar to the phenomenon reported by Matsuo and Ozawa [9]. Further, the experiment values fall - 182 - 0.32 95% confidence interval of coarse grain 0.30 0.28 Vglim' of coarse grain Mesured（Fine） Mesured（Coarse） Analyzed（Fine） Analyzed（Coarse） 0.26 95% confidence interval of fine grain Obstacle condition: R2 0.40 3 3 0.34 3 3 Vglim' of fine grain 0.41 Vglim(m /m ) 0.36 Vglim (m /m ) Maximum coarse aggregate content, 0.42 Obstacle condition: R1 Maximum coarse aggregate content, 95% confidence interval of fine grain 0.38 0.39 0.38 Vglim' of fine grain 0.37 95% confidence interval of coarse grain 0.36 0.35 Mesured（Fine） Mesured（Coarse） Analyzed（Fine） Analyzed（Coarse） Vglim' of coarse grain 0.34 0.33 20 30 40 50 60 70 80 Mean net opening between bars D10, L 0 （mm） 20 30 40 50 60 70 Mean net opening between bars D13, L 0 （mm） 80 Fig. 20 Comparison between measured and analyzed values (obstacle condition R2) Fig. 19 Comparison between measured and analyzed values (obstacle condition R1) Table 6 Analysis parameters Obstacle condition R1 R2 Grading θ Fine grain Coarse grain Fine grain Coarse grain 3.57 5.36 3.57 5.36 Coarse aggregate quality Mean Mean diameter p aspect ratio d50 (mm) 1.63 8.2 1.45 1.57 9.8 1.47 1.63 8.2 1.45 1.57 9.8 1.47 Analysis parameters Mortar properties Thickness of adhering Density Yield value mortar film 3 (Pa) (g/cm ) t 50 (mm) 2.04 13 0.8 2.09 19 1.0 2.02 9 0.5 2.05 11 0.7 Bar obstacle condition Mean net Bar opening diameter L 0 (mm) φ(mm) Concrete film thickness c (mm) 35 10 6.5 40 13 7.0 within the 95% confidence interval of the analytical values, suggesting that use of the space blocking model to estimate Vglim, as proposed in this paper, is applicable to any grading. Influence of obstacle conditions The influence of coarse aggregate particle size distribution under the obstacle conditions specified by the JSCE test method [7] was investigated in the previous section. However, the variations in bar spacing and bar diameter specified in this test method are not as great as those found in actual structures. D19 190 3.2 [in mm] 200 35 35 35 35 53 Type: US1 D16/2 D16 D16 59 53 Type: US2 83 83 Type: US3 Fig.21 Bar obstacle conditions in U-type tester Sakamoto et al. [33],[34] conducted experiments on the effects of obstacle conditions and coarse aggregate content on the self-compactability of combination-type self-compacting concrete using three widely different bar spacings. Their results are illustrated in Fig. 21. The applicability of the space blocking model to any given obstacle conditions is investigated in the following sections based on this experimental data reported by Sakamoto et al. a) (i) Parameter setting for space blocking model Particle size distribution Since no grading data are given in the Sakamoto report, an assumed particle size distribution was adopted for the coarse aggregate (Gmax = 20 mm), as shown in Fig. 22. This was estimated from the measurements of fineness modulus (6.70) by adopting a particle size distribution corresponding to the fineness modulus assumed in the range of standard grading specified in JIS A 5005. Values of θ = 4.19 and p = 1.35 were selected as the parameters in - 183 - Mean aspect ratio of coarse aggregate, a/b Percentage passing by weight (%) 100 90 80 70 60 50 40 30 20 10 0 Range of standard grading by JIS A 5005 0 1.60 1.55 Place of production A： Ohme B： Iwase C： Tsukuba D： Kasama E： Teine River gravel： Kinugawa B 1.50 1.45 E C Crushed stone River gravel 1.40 D 1.35 R2 = 0.765 A River gravel 1.30 56 58 60 62 64 66 68 Solid volume percentage of coarse aggregate, Glim(%) 5 10 15 20 25 30 Nominal size of sieve opening (mm) Fig. 22 Estimated grading of coarse aggregate Fig. 23 Relationship between solid volume percentage and mean aspect ratio of coarse aggregate Eq. (3) for this particle size distribution. The mean diameter of the coarse aggregate according to the number-based distribution is 8.8 mm. (ii) Mean aspect ratio Figure 23 shows the relationship between solid volume percentage and mean aspect ratio based on data presented by Iwai et al. (given as the “square ratio” in the original text) [35] as well as on data by the authors (average of fine-grain and coarse-grain types). Given the good correlation between the solid volume percentage and aspect ratio of crushed stone, the mean aspect ratio is estimated from the solid volume percentage using Eq. (21) (Solid volume percentage = 60.3%, mean aspect ratio = 1.40). a / b = − 0 .0401 G lim + 3 .82 where (iii) (21) a b = mean aspect ratio of coarse aggregate Glim = solid volume percentage of coarse aggregate (%) Mortar properties Sakamoto et al. measured the yield value of mortar wet-screened from concrete. Since the yield value of the mortar for each set of obstacle conditions is not specifically reported, the average of all mixtures (C4-C7 in the original text) is adopted. The mortar yield value and density are therefore assumed to be 15 Pa and 2.10 g/cm 3 , respectively. These values are substituted into Eq. (13) to calculate the film thickness of mortar adhering to the bars, t 5 0 (= 0.8 mm). (iv) Film thickness of concrete The thickness of the concrete film bound to as follows: Obstacle condition US1 (Lo = 35 mm, bar Obstacle condition US2 (Lo = 55 mm, φ = Obstacle condition US3 (Lo = 83 mm, φ = the reinforcing bars is calculated using Eq. (17) diameter ( φ ) = 19 mm): c = 7.7 mm 16 mm): c = 7.4 mm 16 mm): c = 7.4 mm - 184 - 0.36 Percentage passing by weight (%) 0.38 95% confidence interval of US2,US3(D16) 3 3 100 95% confidence interval of US1 (D19) Vglim(m /m ) Maximum coarse aggregate content, 0.40 0.34 Vglim' of US2,US3 Mesured 0.32 Vglim' of US1 Analyzed (US1) Analyzed （US２，US3） 90 FM=7.1 Gmax=25 80 70 FM=6.7 Gmax=20 60 50 FM=6.1 Gmax=10 40 30 20 Range of standard grading by JIS A 5005 10 0 0.30 20 0 40 60 80 100 Mean net opening between bars, L 0 （mm） Fig. 24 Comparison between measured and analyzed 5 10 15 20 25 30 35 40 Nominal size of sieve opening (mm) Fig. 25 Grading of coarse aggregate used in analysis values in the literature b) Comparison of space blocking model and measurements Figure 24 compares the coarse aggregate content that results in a fill height of 30cm in a U-type tester (maximum coarse aggregate content) with estimates obtained using the space blocking model. The measurements for all obstacle conditions fall mostly within the 95% confidence interval of the analytical values, suggesting that the space blocking model proposed by the authors is applicable to the estimation of Vglim under any given bar conditions. The self-compacting concrete used in the Sakamoto experiments was not a powder type as used by the authors but a combination type. The proposed method is applicable to these differing types of self-compacting concrete because mortar properties are treated as physical quantities in the model. In consideration of a safety factor, self-compacting concrete can be proportioned by adopting the lower limit of the 95% confidence interval of Vglim (allowable maximum coarse aggregate content, Vglim’) estimated using the space blocking model. 4. INFLUENCE OF VARIOUS FACTORS ON Vglim The validity of the space blocking model was verified in the previous chapter, and its applicability was confirmed. In this chapter, assessment of the influence of various factors on Vglim is carried out using the space blocking model. The concrete slump flow, grading (fineness modulus), and solid volume percentage of coarse aggregate as well as the obstacle conditions were selected as factors affecting Vglim based on the results already described. The method of assessing the degrees of influence of each factor is as described below. Three different gradings are adopted, as shown in Fig. 25. The mean aspect ratio is determined from Eq. (21) in regard to the range of solid volume percentage between 57% and 62%. As obstacle conditions, the net opening between bars is 35 mm to 200 mm and the bar diameter is D10 to D19 so as to simulate standard self-compacting concrete placed in situ. It is necessary to establish mortar properties for the analysis such that the slump flow - 185 - Table 7 Analysis cases Analysis condition 650 6.1 600 650 6.7 600 650 7.1 600 D10 D13 D10 D13 D10 D13 D10 D13 D10 D13 D10 D13 35 (R1) 40 (R2) 35 (R1) 40 (R2) 35 (R1) 40 (R2) 35 (R1) 40 (R2) 35 (R1) 40 (R2) 35 (R1) 40 (R2) Analysis parameter Glim of coarse aggregate (%) 59 57 59 57 59 57 59 57 59 57 59 57 θ p d 50 (mm) 2.90 3.40 7.6 τm (Pa) 12 21 12 4.19 1.35 8.8 2.08 21 12 5.77 1.28 10.3 21 falls within the self-compacting range. The yield value of the mortar is therefore determined by using the relationship between mortar flow and slump flow (Eq. (22)) established from previous test results [10], as shown in Fig. 26, and substituting the result into Eq. (20). The average density of all mixtures in Fig. 26, that is 2.08 g/cm 3 , is adopted as the density. However, the mortar yield value is established so as to correspond to a slump flow within the range Sf = 600-650 mm, since concrete tends to segregate when the slump flow exceeds 650 mm in Fig. 26. Fm = 0 .324 Sf + 87 .6 ωm (g/cm3) (22) 4.1 a/b 0.7 0.7 1.1 1.1 0.7 0.7 1.1 1.1 0.7 0.7 1.2 1.1 1.45 1.53 1.45 1.53 1.45 1.53 1.45 1.53 1.45 1.53 1.45 1.53 φ (mm) c (mm) Le (mm) h (mm) 10 13 10 13 10 13 10 13 10 13 10 13 6.5 7.0 6.5 7.0 6.5 7.0 6.5 7.0 6.5 7.0 6.5 7.0 22 26 22 26 22 26 22 26 22 26 22 26 190 Vg 0.28 Fine Vg 0.28 M iddle Vg 0.28 Coarse Vg 0.30 Coarse Vg 0.32 Fine Vg 0.32 M iddle Vg 0.32 Coarse Vg 0.36 Fine Vg 0.36 M iddle Vg 0.36 Coarse 340 320 300 280 260 R2 = 0.954 240 220 200 M ean density of mortar calculated from mix 180 proportions=2.08g/cm3 160 200 where t 50 (mm) 360 Mortar flow, Fm (mm) Mean net FM of Slump flow Reinforcing opening coarse Sf (mm) bar size L 0 (mm) aggregate Fm = mortar flow of wet-screened mortar (mm) Sf = slump flow of concrete (mm) 300 400 500 600 700 800 Slump flow, Sf (mm) Fig. 26 Relationship between slump flow and mortar flow Influence of slump flow and fineness modulus The analysis cases described in Table 7 are compared to assess the influence of concrete slump flow and coarse aggregate grading (fineness modulus) on Vglim. The analysis result for each obstacle condition is shown in Figs. 27 and 28. The allowable maximum coarse aggregate content, Vglim’, refers in the figure to the maximum coarse aggregate content at which self-compactability is maintained (that is, the lower limit of the 95% confidence interval of Vglim). These figures reveal that Vglim’ strongly depends on the slump flow but is scarcely affected by the fineness modulus. Accordingly, when proportioning for a target slump flow of, e.q., 650 mm, it is recommended that a Vglim’ value corresponding to a 600 mm slump flow (that is, a 50 mm reduction) be selected to be on the safe side, as a 600 mm slump flow is regarded as being within the quality tolerances. An investigation is carried out to assess the influence of fineness modulus in detail. Figure 29 shows the relationships between Vglim and Vglim’ used in calculating the values in Fig. 27. This figure reveals that Vglim’ has the same value regardless of variations in fineness modulus, whereas the average and confidence interval of Vglim decrease as the fineness modulus of the coarse aggregate decreases. The relationships among void percentage, apparent mortar adherence ratio, and standard deviation of packing ratio corresponding to the fineness modulus used in calculating the values in Fig. 29 are shown in Fig. 30. This figure reveals that, as the fineness increases, the - 186 - Range recommended recommended Range JSCE Guidelines Guidelines by JSCE 0.30 0.30 JIS A 5005(2005,2505) 5005(2005,2505) 0.25 0.25 Obstacle condition: R1(Glim=59%) 0.20 0.20 0.40 0.40 0.35 0.35 Obstacle condition: R2(Glim=57%) 0.20 0.20 95% confidence confidence 95% interval of of Vglim Vglim interval Allowable maximum maximum coarse Allowable aggregate content, Vglim' coarse aggregate content, 1.96 σpf 1.96 σpf a/b a/b Void percentage, ε Apparent adhering mortar ratio, δm Maximum Maximumcoarse coarse aggregate aggregate content, content, 3 3 Vglim /m3)) (m3/m Vglim (m Obtacle conditions: Obtacle conditions: R1 R1 Average Average of Vglim Vglim of 0.20 Fig. 28 Effect of slump flow and fineness modulus, R2 0.40 Sf=600mm =600mm Sf a/b =1.45(Glim =1.45(Glim=59%) =59%) a/b 0.30 0.30 0.25 JIS JIS A A 5005(2005,2505) 5005(2005,2505) 0.25 0.25 5.0 6.0 7.0 8.0 5.0 6.0 Fineness modulus of coarse aggregate, FM Fineness modulus of Fig. 27 Effect of slump flow and fineness modulus, R1 0.35 0.35 Range Range recommended recommended by by JSCE JSCE Guidelines Guidelines 0.30 0.30 6.0 7.0 8.0 5.0 7.0 8.0 Fineness modulus of coarse aggregate, aggregate, FM FM 0.40 0.40 Sf=650mm Sf=650mm Sf=600mm Sf=600mm V li ' 0.35 0.025 0.30 0.020 0.25 0.015 0.20 0.010 ε（Sf=600mm） δm（Sf=600mm） 0.15 0.005 σpf(Sf=600mm) 0.10 6.0 7.0 8.0 5.0 6.0 7.0 8.0 Fineness modulus modulus of of coarse coarse aggregate, aggregate,FM FM Fineness Fig. 29 Relationship between Vglim and Vglim' 0.030 Packing ratio of coarse aggregate particles 0.000 5.0 6.0 7.0 Standard deviation of packing ratio PF, σpf 0.35 0.35 Sf=650mm Sf=600mm Allowable maximum maximumcoarse coarse aggregate aggregate Allowable 33 33 /m )) content,Vglim' Vglim' (m (m /m content, Allowable maximum coarse aggregate aggregate 3 3 content, Vglim' (m3 /m3)) 0.40 0.40 8.0 Fineness modulus of coarse aggregate, FM Fig. 30 Analyzed void percentage, apparent mortar adherence ratio, and standard deviation of packing ratio void percentage falls due to the wall effect, but the apparent mortar adherence ratio increases. This kind of increase in apparent mortar adherence ratio with respect to the opening cross section generally means that, with increasing particle fineness, the specific surface increases, thereby increasing the adherence for a given set of mortar properties. Therefore it can be deduced that the influences of void percentage, apparent mortar adherence ratio, and standard deviation of the packing ratio offset one another at each fineness modulus, leading to an apparent absence of influence of fineness modulus on Vglim’. Accordingly, the influence of coarse aggregate fineness modulus on Vglim’ is considered marginal for a given slump flow. Variations in maximum coarse aggregate content noted with different gradings are thought to result from differences in slump flow (mortar flow). According to the JSCE Recommendations [7], the appropriate coarse aggregate content for self-compactability ranges from 0.28 to 0.30 m 3 /m 3 (Sf = 600-700 mm) when the solid volume percentage is 59% or more under obstacle condition R1. Under obstacle condition R2, the recommended coarse aggregate content is 0.30 to 0.33 m 3 /m 3 (Sf = 600-700 mm) when the solid volume percentage is 57% or more. These recommended ranges of coarse aggregate content correspond to the lower and upper values of analytical results with R1 and R2 (Figs. 27 and 28), respectively, both of which fall within the range estimated using the space blocking model. - 187 - Table 8 Analysis cases Analysis parameter 35 (R1) D10 6.7 60 125 600 200 0.38 4.19 1.35 0.34 3 3 35 60 200 p θ Sf=600mm FM=6.7 0.36 Vglim' (m /m ) Allowable maximum coarse aggregate content, D19 Glim of coarse aggregate (%) 59 62 59 62 59 59 62 59 59 59 0.32 0.30 Glim=59% 0.28 Glim=62% d50 (mm) 8.8 Void percentage, ε Apparent adhering mortar ratio, δm Mean net FM of Slump flow Reinforcing opening coarse Sf (mm) bar size L0 (mm) aggregate 0.26 0 50 100 150 200 (Pa) 21 t50 (mm) a/b 1.1 1.1 1.1 1.1 1.1 1.1 1.1 1.1 1.1 1.1 1.45 1.33 1.45 1.33 1.45 1.45 1.33 1.45 1.45 1.45 φ (mm) c (mm) Le (mm) 10 47 6.5 112 19 20 45 185 7.7 0.025 0.36 0.020 Packing ratio of coarse aggregate particles PF =1-ε-δ m 0.015 0.28 0.010 0.24 0.005 0.000 50 100 190 187 ε（Glim=59%) δm（Glim=59%） σpf（Glim=59%） 0.32 h (mm) 22 0.40 0 Mean net opening between bars D10, L 0 (mm) 4.2 2.08 τm 0.20 250 Fig. 31 Effects of solid volume ratio and mean net opening between bars ωm (g/cm3) 150 200 250 Standard deviation of packing ratio PF, σpf Analysis condition Mean net opening between bars D10, L 0 (mm) Fig. 32 Analyzed void percentage, apparent mortar adherence ratio, and standard deviation of packing ratio Influence of solid volume percentage and obstacle conditions Vglim’, is calculated for each analysis case shown in Table 8 for a fixed the slump flow of Sf = 600 mm and a fineness modulus of FM = 6.7, so as to investigate the influence of coarse aggregate solid volume percentage and obstacle conditions. The results are shown in Fig. 31. This figure shows that Vglim’ increases as the mean net opening between bars increases and the solid volume percentage of coarse aggregate increases. The wider the mean net opening between bars becomes, the smaller its influence on Vglim’ tends to be, and there is an abrupt change at around 60 mm. The JSCE Recommendations [7] adopt 60 mm as the threshold value between Rank 1 and Rank 2 bar arrangement conditions (minimum clearance between bars). The relationships between void percentage, apparent mortar adherence ratio, and standard deviation of the packing ratio and the mean net bar opening are investigated to assess in detail the influence of mean net opening of the reinforcing bars. As shown in Fig. 32, the void percentage gradually decreases and converges to a certain value as the mean net opening increases. This is similar to the phenomenon observed in powder engineering, in which the void percentage of particles with a fixed diameter gradually decreases and levels off at a certain value when the container size increases [15]. The present results therefore confirm the existing theory. Figure 33 shows the influence of bar diameter on Vglim’. This figure shows that Vglim’ decreases as the bar diameter increases for a given mean net opening, but that the influence of bar diameter is not as great as that of mean net opening. Miura et al. reported that the - 188 - 0.38 0.36 3 3 Vglim' (m /m ) Allowable maximum coarse aggregate content, ability of concrete to pass through a narrow opening decreases as the diameter of the bars increases even as the mean net opening remains the same [36]. The space blocking model appears to reflect this phenomenon properly. 0.34 0.32 Sf=600mm These results demonstrate that mortar FM=6.7 0.30 Glim=59% properties (slump flow), mean net opening between bars, and solid volume percentage are D10 0.28 predominant factors affecting Vglim’. Further, D19 the coarse aggregate content in the JSCE 0.26 Recommendations [7] is specified on the basis 0 50 100 150 200 250 of a great deal of construction experience and Mean net opening between bars, L 0 (mm) experimental data, with slump flow, bar obstacle conditions, and solid volume Fig. 33 Effect of bar diameter and mean net opening percentage taken as the key factors, and this also confirms the validity of the estimation model for Vglim proposed here. The threshold between bar arrangement conditions for self-compactability Rank 1 and Rank 2 agrees with the estimation given by this model, and this also proves the validity of the proposed model. 5. CONCLUSIONS The limit state of self-compactability was assumed to be when bridging of coarse aggregate particles covered with a mortar film occurs. A space blocking model was then formulated by applying a probability model based on a Monte-Carlo simulation to the particle size distribution of coarse aggregate and the bridge structure. The validity of the model was assessed by comparison with studies in the literature, and this verified the proposed model. The model was also proven valid by comparison with the JSCE Recommendations. It is therefore concluded that the maximum coarse aggregate content, Vglim, can be estimated from the coarse aggregate quality (grading and mean aspect ratio) and mortar properties (yield value and density) by using the model under any given obstruct conditions caused by the bar arrangement in a U-type self-compactability tester. The mean aspect ratio and yield value of the mortar phase of the concrete require future investigation in order to improve the accuracy of the model and simplify the calculations. The authors also intend to investigate the relationship between mean aspect ratio and solid volume percentage, as well as the relationship between mortar phase yield value and the flow of mortar mixed without coarse aggregate. Since this study has made clear which mortar properties affect the limit state of self-compactability, the mortar proportioning factors that lead to such properties will also be investigated in relation to self-compactability. These will include the water-powder ratio, powder qualities, chemical admixture dosage, fine aggregate quality, and fine aggregate content. References [1] K.Takada, J.C.Walraven and W.Bennenk: Self-Compacting Concrete in the Netherlands, Concrete Journal, JCI, Vol.38, No.3, pp.17-23, 2000. [2] I.Izumi: High Fluidity Concrete, Concrete Journal, JCI, Vol.36, No.11, pp.41-43, 1998. [3] T.Nawa, H.Eguchi, M.Okubo and Y.Fukaya: A Discussion on Mix Design and Fluidity of Self-compacting Concrete, Proceedings of JCI, Vol.14, No.1, pp.369-374, 1992. [4] A.Dozono, H.Fujiwara and Y.Shimoyama: A Study on Passability of Self-compacting Concrete between Reinforcing Bars, Proceedings of JSCE Annual Conference, Vol.Ⅴ, pp.308-309, 1994. - 189 - [5] H.Okamura and K.Ozawa: Mix Design Method for Self-Compactable Concrete, Journal of Materials,Concrete Structures and Pavements, JSCE, No.496/V-24, pp.1-8, 1994. [6] Recommendations for Mix Design and Construction Practice of Highly Fluid Concrete, Architectural Institute of Japan, 1997. [7] Recommendations for Construction of Self-compacting Concrete Structures, Concrete Library 93, JSCE, 1998. [8] Committee Report – Super Flowing Concrete (I), JCI, pp.12-18, 1993. [9] S.Matsuo and K.Ozawa: Effect of Coarse Aggregate Properties on the Filling Capacity of Self-compacting Concrete, Proceedings of JCI, Vol.16, No.1, pp.165-170, 1994. [10] J.Ogihara, T.Nawa, M.Nakai and T.Saito: Influence of Grading and Content of Coarse Aggregate on Self-Compactability of Self-Compacting Concrete, Cement Science and Concrete Technology, No.53, pp.397-402, 1999. [11] T.Noguchi, F.Tomozawa and X.Wu: A Rheological Discussion on Passability through Narrow Spaces of Self-compacting Concrete, Proceedings of JCI, Vol.17, No.1, pp.23-28, 1995. [12] C.Saito, R.Chikamatsu, A.Yonemura and A.Yamada: Effect of Coarse Aggregate on Self-compactability of Self-compacting Concrete, Proceedings of JSCE Annual Conference, Vol.Ⅴ, pp866-867, 1997. [13] H.Fujiwara, S.Nagataki, N.Otsuki and A.Dozono: Study on the Ability to Pass between Steel Reinforcing Bars of Highly Flowable Concrete, Journal of Materials,Concrete Structures and Pavements, JSCE, No.550/V-33, pp.23-32, 1996. [14] H.Mori and Y.Tanigawa: The State of the Art on Flow Analysis of Fresh Concrete, Concrete Journal, JCI, Vol.32, No.12, pp.30-40, 1994. [15] S.Miwa: Powder Engineering, The Nikkan Kogyo Shimbun Ltd., pp.36-39, 1981. [16] Editorial Committee for Basics of Powder Engineering, Basics of Powder Engineering, The Nikkan Kogyo Shimbun Ltd., pp.31-46, 1992. [17] C.Minoya: Useful Statistical Distributions, Tokyo Tosho Inc., pp.237-243, 1998. [18] K.Wakimoto: Statistics – Aspects and Concept, Nippon Hyoronsha Publishers, pp.107-109, 1984. [19] C.Minoya: A Guide to Statistics 2, Tokyo Tosho Inc., pp.330-335, 1994. [20] T.Midorikawa and K.Maruyama: Evaluation of Particle Shape and Size Distribution of Powder on Water Retention, Journal of Materials, Concrete Structures and Pavements, JSCE, No.544/V-32, pp.121-130, 1996. [21] Committee Report – Research Committee for Mechanical Models of Fresh Concrete, JCI, pp.15, 1996. [22] A Fundamental Study on Quantification of Segregation of Plain Concrete, Cement Science and Concrete Technology, No.43, pp.168-173, 1989. [23] S.Ota: A Study on Investigation and Application of Mixture by Surface Area and New Surface Area of Aggregate, Transactions of JSCE, No.61, Separate Vol.3-3, pp.1-48, 1959. [24] R.Komura, Y.Tanigawa, H.Mori, Y.Kurokawa and Y.Cai: Study on Slumping Behavior of Fresh Concrete (Part1: Estimating Method of Rheological Constants), Summaries of Technical Papers of Annual Meeting Architectural Institute of Japan, pp.519-520, 1994. [25] Y.Arai: Material Chemistry of Powder, Baifukan Co., pp.1-23, 1987. [26] M.Sese and Y.Kawamura: A Guide to Monte Carlo Simulation – Application of Stochastic Simulation to Chemical Industry/Simulation of Random Events (Part 1), Chemical Engineering, No.9, pp.67-74, 1993. [27] K.Ito, Y.Wanibe and H.Sakao: A Simulation of the process of Random Packing of Graded Powder and Analysis of the Packing Structure, Journal of Japan Institute of Metals, Vol.50, No.4, pp.423-429, 1986. [28] Y.Wakayama: Visual Basic for Students, Tokyo Denki University Press, 1998. [29] K.Kato: Visual Basic Programming in an Excel Environment, Kyoritsu Shuppan Co., 1999. [30] T.Suga and M.Hiyama: A Book of Easy Statistics – Manabu, Gendai-Sugakusha, pp.61-65, 1995. - 190 - [31] M.Sese and Y.Kawamura: A Guide to Monte Carlo Simulation – Application of Stochastic Simulation to Chemical Industry/Random Numbers (Part 2), Chemical Engineering, No.1, pp.97-103, 1993. [32] K.wakimoto, T.Tarumi and Y.Tanaka: A Handbook for Statistical Analysis with a Personal Computer/I Basic Statistics, Kyoritsu Shuppan Co., pp.179-195, 1984. [33] J.Sakamoto, K.Yokoi and T.Shindo: Effect of Powder/Coarse Aggregate Content on Self-compactability of Self-compacting Concrete, Proceedings of JCI, Vol.20, No.2, pp.415-420, 1998. [34] K.Yokoi, T.Shindo, J.Sakamoto and K.Yokota: Effect of Mix Constituent on Self-Compactability in Super Workable Concrete “Bio-Concrete”, Taisei Technical Research Report, No.30, pp.59-64, 1997. [35] N.Iwai, Y.Masuda and M.Abe: Effect of Shape and Size of Aggregate on the Properties of Self-compacting Concrete while Fresh, Proceedings of JCI, Vol.18, No.1, pp.117-122, 1996. [36] R.Miura, R.Chikamatsu and S.Togawa: A Suggestion on The Mix Design Method of Self-compacting Concrete, Proceedings of The Self-compacting Concrete Symposium, Concrete Technical Series of JSCE, No.10, pp.59-64, 1996. - 191 -